Continuum mathematics at the nanoscale
© Myers et al.; licensee Springer. 2014
Received: 19 December 2013
Accepted: 18 August 2014
Published: 8 September 2014
In this paper we discuss three examples where continuum theory may be applied to describe nanoscale phenomena:
1. Enhanced flow in carbon nanotubes (CNTs) – This model shows that the experimentally observed enhancement can be explained using standard flow equations but with a depletion layer between the liquid and solid interfaces.
2. Nanoparticle melting – Nanoparticles often exhibit a sharp increase in melting rate as the size decreases. A mathematical model will be presented which predicts this phenomena.
3. Nanofluids – Experimental results concerning the remarkable heat transfer characteristics of nanofluids are at times contradictory. We develop a model for the thermal conductivity of a nanofluid, which provides much higher predictions than the standard Maxwell model and a better match to data.
Keywordscarbon nanotubes enhanced flow nanoparticle melting thermal conductivity nanofluid
Continuum theory may be applied when there is a sufficiently large sample size to ensure that statistical variation of material quantities, such as density, is small. For fluids the variation is often quoted as 1% . Assuming a spherical sample Nguyen and Werely  suggest this level of variation requires a minimum of 104 atoms and so deduce a critical dimension of the order 10 and 90 nm for liquids and gases respectively. In fact by comparing molecular dynamics (MD) simulations to computations based on the Navier-Stokes equations Travis et al.  show that continuum theory may be applied to water flow down to around 3 nm. Thomas et al.  suggest a figure of 1.66 nm. In the field of heat transfer and phase change it has been suggested that continuum theory requires particle radii greater than 2 nm . Kofman et al.  state that at scales smaller than 5 nm the melting process is discontinuous and dominated by fluctuations, Kuo and Clancy  observed structural changes and a ‘quasi-molten’ state in their study of nanoparticle melting between 2-5 nm.
Nanoscale is typically described as involving materials with at least one dimension below 100 nm , so there is clearly a range of sizes where continuum theory may be applied to nano phenomena. In this paper we will discuss work carried out in the Industrial Mathematics Group at the Centre de Recerca Matemàtica using continuum theory to study problems in fluid and heat flow and demonstrate how seemingly anomalous behaviour may be explained without resorting to molecular dynamics or empirically based adjustments. Full details of the group’s work in this area may be found in [9–14]. In Section 2 we will examine the issue of enhanced flow in carbon nanotubes. Many experiments have shown that when water flows through a carbon nanotube the flow rate is orders of magnitude higher than predicted by classical theory. Early papers [15, 16] quote factors of around 4 orders of magnitude, although more recent experiments have shown the true figure is closer to 1 order . In our model we employ a concept taken from non-Newtonian fluid dynamics, that of a bi-viscosity fluid, to explain why observed flow rates of water in carbon nanotubes are much higher than that predicted by classical theory. The model also suggests a physical interpretation for the Navier slip condition. In Section 3 we investigate the melting of nanoparticles. As the particles decrease in size, and so the ratio of bulk to surface atoms decreases, it becomes easier for surface atoms to leave the particle. This results in a decrease in the melt temperature. Using a form of the Gibbs-Thompson relation to describe the variation of melt temperature with size we produce a model that explains the experimentally observed ‘abrupt melting’. The final problem concerns nanofluids, these are fluids containing a suspension of nanoparticles. They have been claimed to significantly increase certain fluid properties, such as the thermal conductivity and heat transfer coefficient. Despite hundreds of papers affirming the remarkable heat transfer properties, it was recently shown in a benchmark study, carried out in over thirty laboratories around the world, that nanofluids do not provide significant improvements . A theoretical demonstration that increasing nanoparticle concentration can decrease heat transfer was shown in . This contradicted many analytical papers using the same model. However, experiments seem clear that the conductivity of the fluids increases significantly with particle concentration. The classical Maxwell model, to describe the heat conduction of a solid-in-liquid suspension, is known to significantly underpredict the thermal response of a nanofluid. In Section 4 we investigate the thermal conductivity of a nanofluid. The Maxwell model is based on a static analysis. Using an approximate solution method to the heat flow problem we obtain an expression for the thermal conductivity of the fluid which shows much better agreement with experiment.
A review on the mathematics of the continuum to describe behaviour at the nanoscale can be found in . Previous mathematical models describing the melting of nanoparticles based on continuum theory exist, for instance [21–23].
2 Enhanced flow in carbon nanotubes
Carbon nanotubes (CNTs) are remarkably strong and light cylindrical nanostructures which are excellent at conducting both heat and electricity. These advantageous properties have led to CNTs being proposed for a diverse range of applications (see ) including DNA gene delivery , biosensor diagnostics , tissue engineering , solar cells  and microelectronics technology (e.g., transistors ). CNTs have also shown promise in the textile field, as they can transport water much quicker than that predicted by classical flow theory. Several authors have shown that by using CNTs, flow can be increased by up to several orders of magnitude [15, 16]. However, more recently Whitby et al.  reported a more conservative maximum increase by a factor of 45. Following the work by Myers , here we demonstrate that the inclusion of a gas depletion layer in the standard flow model accounts for the aforementioned enhanced increase in flow.
Flow enhancement is generally defined as, , the ratio of the observed to predicted fluxes, and thus has an obvious effect on any enhancement in the flow. On the microscale, it has been shown experimentally, that the slip length is much smaller than the channel dimension. In contrast, the slip length for nanochannels is usually of the order of microns. At present, there is no accepted theory for the slip length of a liquid flowing past a solid surface. However, there is one for gases, and the slip length is of the order of the mean free path of the gas . Holt et al.  and Majumder et al.  report slip lengths of the order of microns to match with their corresponding experimental treatments. However, some authors [31, 32] have questioned the validity of the slip modified Hagen-Poiseuille model based on the larger slip lengths reported in CNT studies. Cottin-Bizonne et al.  suggest that the slip length should have a single, radius-independent value and be much smaller than those typically quoted in the literature. In addition, they postulate that the contamination by hydrophobic particles to be the cause of some of the high experimental values. The hydrophobicity of CNTs has been proposed as an alternative explanation to the slip length. Eijkel and van den Berg  report that the strength of attraction between water molecules is greater than the attractive force between the hydrophobic solid and the water. This hydrophobicity can then lead to some form of ‘depletion layer’ which may be interpreted as a region of low viscosity close to the tube wall. Experimentally this may be viewed in terms of ‘apparent’ slip [34, 35]. Several authors have observed this phenomenon experimentally [36–38] and via molecular dynamics simulations .
where , denote the bulk and depletion layer viscosities, respectively, such that . Experimental studies on CNTs indicate a depletion later thickness of , and thus . The flow enhancement is defined as the ratio . If we take experimental data from Whitby et al.  we obtain . Two readily available gases, air and oxygen, have viscosities approximately 0.02 that of water.
For sufficiently wide tubes where we have , and there is no noticeable flow enhancement. As a result the no-slip boundary condition is sufficient. Slip is not observed in wide tubes with smooth surfaces. This condition holds for .
- 2.For moderate tubes where is but then only the leading order term of applies and(6)
For very small tubes where is we require the full expression for , and thus the slip length varies with R.
The R bounds for the different regimes are chosen such that there is a maximum error of 5% when using the approximation.
The present model predicts for which is corroborated by Thomas et al.  who report . The model also predicts a maximum enhancement (obtained by setting ) of approximately 50 which agrees with the maximum value of 45 recorded by Whitby et al. .
3 Nanoparticle melting
Nanoparticles have a large ratio of surface to volume atoms which can have a significant impact on the material properties . One example where this manifests itself is in the well-known decrease in phase change temperature that accompanies a decrease in material dimensions . The experimental treatment of Buffat and Borel  documented a decrease of approximately 500 K for gold particles with radius slightly greater than 1 nm. Similarly, the MD simulations of Shim et al.  demonstrated a decrease of more than 800 K below the bulk melt temperature for gold nanoparticles with a radius around 0.8 nm. This interesting property has resulted in nanoparticles being the subject of research for applications which require the particles to melt after serving their primary purpose, and so pass through the system as disperse molecules. Drugs with poor water solubility may be administered as nanoparticles to improve their uptake. Bergese et al.  and Liu et al.  consider antibiotic and antianginal drugs, which exhibit a melting point depression of around 30 K. Since gold has low toxicity, gold nanoparticles also make good carriers for drug and gene delivery . Hence, an accurate model to understand the thermal behaviour of a nanoparticle and its probable phase change behaviour is extremely desirable. In this section we present a mathematical model describing the melting process of nanoparticles proposed by Font and Myers .
This model is similar to that described in : the main difference being that our Gibbs-Thomson relation includes Δc. As will be seen later, for large particles this does not greatly affect the results but becomes increasingly important as the particle size decreases.
where is the temperature change (with the temperature applied at the nanoparticle surface) and the initial particle radius.
The initial conditions for the above coupled system of equations is and , where the latter value is fixed by solving (10) with . Hence, the problem has been reduced considerably from a system of two heat equations in the solid and liquid defined over a changing domain specified by the Stefan condition and coupled to an equation describing the phase change temperature to solving two first order ODEs.
4 Thermal conductivity of nanofluids
The enhanced thermal properties of nanofluids, compared to their base fluids, has led nanofluids to being an attractive solution for heat removal in modern electronic devices [46, 47]. Consequently, the study of the thermal properties of nanofluids is an intense research area. One of the critical ongoing issues is the lack of a satisfactory theoretical model for the thermal response of a nanofluid [18, 48].
where , , denote the effective, particle and liquid thermal conductivity and ϕ is the particle volume fraction. The Maxwell model has several well-known drawbacks. Foremost, the model is only applicable to heat flow in the material surrounding an equivalent fluid or around a particle, and not the scenario of interest, namely, an actual nanofluid or particle. Secondly, the theory is based on an infinite region  and hence is only applicable to very dilute solutions where the particles are sufficiently far apart such that there is negligible thermal interaction between the particles. Clearly, this will lead to problems if the particle concentration increases. In addition, Maxwell’s theory is based on a steady-state analysis, which restricts one from considering the more interesting time dependent thermal response of the nanofluid.
Despite the aforementioned limitations, the Maxwell model works well for low volume fraction fluids with relatively large particles. However, the accuracy of the model deteriorates when the particle size decreases to the nanoscale. Keblinski et al.  compared experimental data from various nanofluid treatments and reported that in most cases with , which is in contrast to the linearised Maxwell model where . To improve the fit between data and theory, numerous authors have proposed extensions to Maxwell’s model including nanolayers (a thin layer of ordered liquid molecules surrounding the particle), particle clustering, nanoconvection and Brownian motion. For example, Prasher et al.  and Koo and Kleinstreuer  modify Maxwell’s result to account for Brownian motion. Yu and Choi  introduce a nanolayer of width 2 nm with a thermal conductivity ten times greater than that of the base fluid. The extensive review of Das et al.  illustrates that with the inclusion of additional effects and new parameters, there is better agreement between experiment and the variants of Maxwell’s theory. In this section we discuss an alternative expression for the thermal conductivity of a nanofluid recently proposed by Myers et al.  that agrees well with experimental data.
where is the time when the particle temperature first rises noticeably above the initial temperature, , and . From [9, 10] the constant is found by minimising the least-squares error when the approximate solution is substituted into the heat equation.
where and . The accuracy of this formula may be verified by comparison with the exact solution (25).
which indicates that the equivalent particle conductivity is independent of the particle conductivity. Note this has been verified experimentally, see [47, 52]. The particle material properties appear through the density and heat, . However, as the ratio is and ϕ is small, this is a weak dependence. Consequently, the effective conductivity is predominantly a function of the liquid conductivity and volume fraction ϕ.
This paper provides a brief overview of three pertinent problems from the nano field. In the first problem we considered a model for fluid flow in carbon nanotubes. At present there is no theory for calculating the slip lengths for a liquid moving over a solid surface. We used an equivalent theory with a depletion layer over a solid surface to obtain an expression for the slip length in terms of the depletion layer thickness and its viscosity. Next, we presented a mathematical model that successfully captured the ‘abrupt melting’ phenomenon of nanoparticles. In particular, the model demonstrated the sharp increase in melting rate as the size of the nanoparticles decreased. Finally, we considered the thermal conductivity of nanofluids, and our analysis led to an expression for solid-in-liquid suspensions, derived in a distinct way to the seminal Maxwell model. The model showed excellent agreement with experimental data for particle volume fractions greater than 1%.
While this work is at the limit of continuum theory, in each case the continuum models demonstrated good agreement with experimental data and provided valuable insight. Moreover, the results of the nanoscale modelling in some cases led to a deeper understanding of the macroscale problems. At present there is great interest in nanotechnology with applications in a wide range of areas. We have presented results for just three specific problems, however the success of the models indicates that there is great scope for applying continuum models at the nanoscale.
The research of TGM was supported by a Marie Curie International Reintegration Grant Industrial applications of moving boundary problems Grant no. FP7-256417 and Ministerio de Ciencia e Innovación Grant MTM2011-23789. VC was also supported through the Marie Curie Grant. FF and MM acknowledge the support of a Centre de Recerca Matemàtica PhD grant.
- Abragall P, Nguyen N-T: Nanofluidics. 1st edition. Artech House, Norwood; 2009.Google Scholar
- Nguyen N-T, Werely ST: Fundamentals and Applications of Microfluidics. 2nd edition. Artech House, Norwood; 2006.MATHGoogle Scholar
- Travis KP, Todd BD, Evans DJ: Departure from Navier-Stokes hydrodynamics in confined liquids. Phys Rev E 1997,55(4):4288–4295. 10.1103/PhysRevE.55.4288View ArticleGoogle Scholar
- Thomas JA, McGaughey AJH, Ottoleo K-A: Pressure-driven water flow through carbon nanotubes: insights from molecular dynamics simulation. Int J Therm Sci 2010,49(2):281–289. 10.1016/j.ijthermalsci.2009.07.008View ArticleGoogle Scholar
- Guisbiers G, Kazan M, Van Overschelde O, Wautelet M, Pereira S: Mechanical and thermal properties of metallic and semiconductive nanostructures. J Phys Chem C 2008, 112: 4097–4103. 10.1021/jp077371nView ArticleGoogle Scholar
- Kofman R, Cheyssac P, Lereah Y, Stella A: Melting of clusters approaching 0D. Eur Phys J D 1999,9(1–4):441–444.Google Scholar
- Kuo C-L, Clancy P: Melting and freezing characteristics and structural properties of supported and unsupported gold nanoclusters. J Phys Chem B 2005, 109: 13743–13754. 10.1021/jp0518862View ArticleGoogle Scholar
- Das SK, Choi SU, Yu W, Pradeep T: Nanofluids: Science and Technology. 1st edition. Wiley, New York; 2008.Google Scholar
- Myers TG: Optimizing the exponent in the heat balance and refined integral methods. Int Commun Heat Mass Transf 2009,36(2):143–147. 10.1016/j.icheatmasstransfer.2008.10.013View ArticleGoogle Scholar
- Myers TG: Optimal exponent heat balance and refined integral methods applied to Stefan problems. Int J Heat Mass Transf 2010,53(5–6):1119–1127. 10.1016/j.ijheatmasstransfer.2009.10.045MATHView ArticleGoogle Scholar
- Myers TG: Why are slip lengths so large in carbon nanotubes? Microfluid Nanofluid 2011,10(5):1141–1145. 10.1007/s10404-010-0752-7View ArticleGoogle Scholar
- Font F, Myers TG: Spherically symmetric nanoparticle melting with a variable phase change temperature. J Nanopart Res 2013.,15(12): Article ID 2086 Article ID 2086 10.1007/s11051-013-2086-3Google Scholar
- Myers TG, MacDevette MM, Ribera H: A time-dependent model to determine the thermal conductivity of a nanofluid. J Nanopart Res 2013.,15(7): Article ID 1775 Article ID 1775 10.1007/s11051-013-1775-2Google Scholar
- Font F, Myers TG, Mitchell SL: A mathematical model for nanoparticle melting with density change. Microfluid Nanofluid 2014. 10.1007/s10404-014-1423-xGoogle Scholar
- Holt JK, Park HG, Wang Y, Stadermann M, Artyukhin AB, Grigoropoulos CP, Noy A, Bakajin O: Fast mass transport through sub-2-nanometer carbon nanotubes. Science 2006,312(5776):1034–1037. 10.1126/science.1126298View ArticleGoogle Scholar
- Majumder M, Chopra N, Andrews R, Hinds BJ: Nanoscale hydrodinamics: enhanced flow in carbon nanotubes. Nature 2005, 438: 44. 10.1038/438044aView ArticleGoogle Scholar
- Whitby M, Cagnon L, Thanou M, Quirke N: Enhanced fluid flow through nanoscale carbon pipes. Nano Lett 2008,8(9):2632–2637. 10.1021/nl080705fView ArticleGoogle Scholar
- Buongiorno J, Venerus DC, Prabhat N, McKrell T, Townsend J, Christianson R, Tolmachev YV, Keblinski P, Hu L-w, Alvarado JL, Bang IC, Bishnoi SW, Bonetti M, Botz F, Cecere A, Chang Y, Chen G, Chen H, Chung SJ, Chyu MK, Das SK, Di Paola R, Ding Y, Dubois F, Dzido G, Eapen J, Escher W, Funfschilling D, Galand Q, Gao J, Gharagozloo PE, Goodson KE, Gutierrez JG, Hong H, Horton M, Hwang KS, Iorio CS, Jang SP, Jarzebski AB, Jiang Y, Jin L, Kabelac S, Kamath A, Kedzierski MA, Kieng LG, Kim C, Kim J-H, Kim S, Lee SH, Leong KC, Manna I, Michel B, Ni R, Patel HE, Philip J, Poulikakos D, Reynaud C, Savino R, Singh PK, Song P, Sundararajan T, Timofeeva E, Tritcak T, Turanov AN, Van Vaerenbergh S, Wen D, Witharana S, Yang C, Yeh W-H, Zhao X-Z, Zhou S-Q: A benchmark study on the thermal conductivity of nanofluids. J Appl Phys 2009.,106(9): Article ID 094312 Article ID 094312Google Scholar
- MacDevette MM, Myers TG, Wetton B: Boundary layer analysis and heat transfer of a nanofluid. Microfluid Nanofluid 2014,17(2):401–412. 10.1007/s10404-013-1319-1View ArticleGoogle Scholar
- Thamwattana N, Hill JM, Baowan D, Cox BJ: A review of mathematical and mechanical modelling in nanotechnology. Math Mech Solids 2010, 15: 708–717. 10.1177/1081286510375344MATHMathSciNetView ArticleGoogle Scholar
- Wu T, Liaw H-C, Chen Y-Z: Thermal effect of surface tension on the inward solidification of spheres. Int J Heat Mass Transf 2002,45(10):2055–2065. 10.1016/S0017-9310(01)00313-1MATHView ArticleGoogle Scholar
- Wu B, McCue SW, Tillman P, Hill JM: Single phase limit for melting nanoparticles. Appl Math Model 2009,33(5):2349–2367. 10.1016/j.apm.2008.07.009MATHMathSciNetView ArticleGoogle Scholar
- McCue SW, Wu B, Hill JM: Micro/nanoparticle melting with spherical symmetry and surface tension. IMA J Appl Math 2009, 74: 439–457. 10.1093/imamat/hxn038MATHMathSciNetView ArticleGoogle Scholar
- Meyyappan M: Carbon Nanotubes: Science and Applications. 1st edition. CRC Press, Boca Raton; 2004.View ArticleGoogle Scholar
- Pantarotto D, Singh R, McCarthy D, Erhardt M, Briand J-P, Prato M, Kostarelos K, Bianco A: Functionalized carbon nanotubes for plasmid DNA gene delivery. Angew Chem, Int Ed Engl 2004,43(39):5242–5246. 10.1002/anie.200460437View ArticleGoogle Scholar
- Wang J: Carbon-nanotube based electrochemical biosensors: a review. Electroanalysis 2005,17(1):7–14. 10.1002/elan.200403113View ArticleGoogle Scholar
- Zanello LP, Zhao B, Hu H, Haddon RC: Bone cell proliferation on carbon nanotubes. Nano Lett 2006,6(3):562–567. 10.1021/nl051861eView ArticleGoogle Scholar
- Suzuki K, Yamaguchi M, Kumagai M, Yanagida S: Application of carbon nanotubes to counter electrodes of dye-sensitized solar cells. Chem Lett 2003,32(1):28–29. 10.1246/cl.2003.28View ArticleGoogle Scholar
- Heinze S, Tersoff J, Martel R, Derycke V, Appenzeller J, Avouris P: Carbon nanotubes as Schottky barrier transistors. Phys Rev Lett 2002., 89: Article ID 106801 Article ID 106801 10.1103/PhysRevLett.89.106801Google Scholar
- White FM: Viscous Fluid Flow. 1st edition. McGraw-Hill, New York; 1991.Google Scholar
- Thomas JA, McGaughey AJH: Reassessing fast water transport through carbon nanotubes. Nano Lett 2008,8(9):2788–2793. 10.1021/nl8013617View ArticleGoogle Scholar
- Verweij H, Schillo MC, Li J: Fast mass transport through carbon nanotube membranes. Small 2007,3(12):1996–2004. 10.1002/smll.200700368View ArticleGoogle Scholar
- Cottin-Bizonne C, Cross B, Steinberger A, Charlaix E: Boundary slip on smooth hydrophobic surfaces: intrinsic effects and possible artifacts. Phys Rev Lett 2005., 94: Article ID 056102 Article ID 056102Google Scholar
- Eijkel JT, van den Berg A: Nanofluidics: what is it and what can we expect from it? Microfluid Nanofluid 2005,1(3):249–267. 10.1007/s10404-004-0012-9View ArticleGoogle Scholar
- Neto C, Evans DR, Bonaccurso E, Butt H-J, Craig VSJ: Boundary slip in Newtonian liquids: a review of experimental studies. Rep Prog Phys 2005,68(12):2859. http://stacks.iop.org/0034–4885/68/i=12/a=R05 http://stacks.iop.org/0034-4885/68/i=12/a=R05 10.1088/0034-4885/68/12/R05View ArticleGoogle Scholar
- Poynor A, Hong L, Robinson IK, Granick S, Zhang Z, Fenter PA: How water meets a hydrophobic surface. Phys Rev Lett 2006., 97: Article ID 266101 Article ID 266101 10.1103/PhysRevLett.97.266101Google Scholar
- Joseph S, Aluru NR: Why are carbon nanotubes fast transporters of water? Nano Lett 2008,8(2):452–458. 10.1021/nl072385qView ArticleGoogle Scholar
- Barrat J-L, Bocquet L: Influence of wetting properties on hydrodynamic boundary conditions at a fluid/solid interface. Faraday Discuss 1999, 112: 119–128.View ArticleGoogle Scholar
- Matthews MT, Hill JM: Nanofluidics and the Navier boundary condition. Int J Nanotechnol 2008,5(2/3):218–242. 10.1504/IJNT.2008.016917View ArticleGoogle Scholar
- Choi C-H, Westin KJA, Breuer KS: Apparent slip flows in hydrophilic and hydrophobic microchannels. Phys Fluids 2003,15(10):2897–2902. 10.1063/1.1605425View ArticleGoogle Scholar
- Shim J-H, Lee B-J, Cho YW: Thermal stability of unsupported gold nanoparticle: a molecular dynamics study. Surf Sci 2002, 512: 262–268. 10.1016/S0039-6028(02)01692-8View ArticleGoogle Scholar
- Buffat P, Borel JP: Size effect on the melting temperature of gold particles. Phys Rev A 1976,13(6):2287–2297. 10.1103/PhysRevA.13.2287View ArticleGoogle Scholar
- Bergese P, Colombo I, Gervasoni D, Depero LE: Melting of nanostructured drugs embedded into a polymeric matrix. J Phys Chem B 2004, 108: 15488–15493. 10.1021/jp048762uView ArticleGoogle Scholar
- Liu X, Yangb P, Jiang Q: Size effect on melting temperature of nanostructured drugs. Mater Chem Phys 2007, 103: 1–4. 10.1016/j.matchemphys.2007.01.014View ArticleGoogle Scholar
- Rana S, Bajaj A, Mout R, Rotello VM: Monolayer coated gold nanoparticles for delivery applications. Adv Drug Deliv Rev 2012, 64: 200–216. 10.1016/j.addr.2011.08.006View ArticleGoogle Scholar
- Nguyen CT, Roy G, Gauthier C, Galanis N: Heat transfer enhancement using Al 2 O 3 -water nanofluid for an electronic liquid cooling system. Appl Therm Eng 2007,27(8–9):1501–1506. 10.1016/j.applthermaleng.2006.09.028View ArticleGoogle Scholar
- Yu W, France DM, Routbort JL, Choi SUS: Review and comparison of nanofluid thermal conductivity and heat transfer enhancements. Heat Transf Eng 2008,29(5):432–460. 10.1080/01457630701850851View ArticleGoogle Scholar
- Prasher R, Bhattacharya P, Phelan PE: Thermal conductivity of nanoscale colloidal solutions (nanofluids). Phys Rev Lett 2005., 94: Article ID 025901 Article ID 025901Google Scholar
- Maxwell JC: A Treatise on Electricity and Magnetism. Volume 1. 3rd edition. Clarendon Press, Oxford; 1881.Google Scholar
- Keblinski P, Eastman JA, Cahill DG: Nanofluids for thermal transport. Mater Today 2005,8(6):36–44. 10.1016/S1369-7021(05)70936-6View ArticleGoogle Scholar
- Koo J, Kleinstreuer C: A new thermal conductivity model for nanofluids. J Nanopart Res 2004,6(6):577–588. 10.1007/s11051-004-3170-5View ArticleGoogle Scholar
- Yu W, Choi SUS: The role of interfacial layers in the enhanced thermal conductivity of nanofluids: a renovated Maxwell model. J Nanopart Res 2003,5(1–2):167–171. 10.1023/A:1024438603801View ArticleGoogle Scholar
- Zhou S-Q, Ni R: Measurement of the specific heat capacity of water-based Al 2 O 3 nanofluid. Appl Phys Lett 2008.,92(9): Article ID 093123 Article ID 093123Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.